International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-1435-1441 ISSN: 2249-6645www.ijmer.com 1435 | PageK. Sridhar, 1R. Reji Kumar, 2M. Narasimha3123Lecturer, School of Mechanical and Industrial Engineering Bahirdar University, Bahirdar, EthiopiaAbstract: The specific outputs of some diesel engine applications have produced thermal loadings in excess of the strengthof typical aluminium piston alloys. Functionally graded coatings are used to increase performances of high temperaturecomponents in diesel engines. Thermal barrier coating are being evaluated to return the components durability toacceptable levels as well as providing a means of lowering heat rejection. This paper discusses the use of a finite elementmodel to analyze these thermal barrier coating systems, including the impact of material properties, coating thickness,residual stress and boundary conditions.These coatings consist of a transition from the metallic bond layer to cermet and from cermet to the ceramic layer.Thermal analyses were employed to deposit metallic, cermet and ceramic powders such as NiCrAl, NiCrAl+MgZrO3 andMgZrO3 on the substrate. The numerical results of AlSi and steel pistons are compared with each other. It was shown thatthe maximum surface temperature of the functional graded coating AlSi alloy and steel pistons was increased by 28% and17%, respectively. In this study, thermal behavior of functional graded coatings on AlSi and steel piston materials wasinvestigated by means of using a commercial code, namely ANSYSKey Words: Zirconia, Mullite, Alumina, Thermal efficiency, Electron Beam Physical Vapour DepositionList of SymbolsSymbol Description UnitNomenclatureH Heat transfer coefficient W/m2/K density Kg/m3A Area mm2Pm Indicated Mean Effective Pressure, N/mm2D Diameter of bore mP Thermal expansion ° C-1N Speed rpmN Number of strokes Strokes/minCp Specific heat capacity J/Kg/KTc Temperature at center of the piston ° CTe Temperature at edge of the piston ° CK Thermal conductivity W/m/KAbbreviationHCV Higher calorific value KJ/KgBP Brake power KWTBC Thermal barrier coatingEBPVD Electron beam physical vapor depositionI. IntroductionThe demand for energy is increasing day by day. The world is depending mostly on fossil fuels to face this energyneeds. The increase in standard of living demands better mode of transport, hence a large number of automobile companieshas been introduced. Automobiles provide better transport but the combustion of fuel in automobile engine creates harmfuleffluents, which has an adverse effect on water and air.Combustion generated pollution is by far the largest man madecontribution to atmospheric pollution. The principal pollutants emitted by the automobile engines are CO, NOX, HC andparticulates. The modern day automobiles is a result of several technological improvements that have happened over theyears and would continue to do so to meet the performance demands of Exhaust-Gas Emissions, Fuel Consumption, PowerOutput, Convenience and Safety.In order to reduce emissions and increasing engine performance, modern car enginescarefully designed to control the amount of fuel they burn. An effective way for reducing automotive emission and increaseengine’s performance is accomplished by coating automobile piston head with low thermal conductivity material such asceramic. This process is known as Thermal Barrier Coating (TBC).ANSYS is general-purpose finite element analysis (FEA) software package. Finite Element Analysis is a numericalmethod of deconstructing a complex system into very small pieces (of user-designated size) called elements. The softwareimplements equations that govern the behaviour of these elements and solves them all; creating a comprehensive explanationof how the system acts as a whole. These results then can be presented in tabulated or graphical forms. This type of analysisis typically used for the design and optimization of a system far too complex to analyze by hand. Systems that may fit intoThermal barrier Analysis in Diesel
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-1435-1441 ISSN: 2249-6645www.ijmer.com 1436 | Pagethis category are too complex due to their geometry, scale, or governing equations.ANSYS is the standard FEA teaching toolwithin the Mechanical Engineering Department at many colleges. ANSYS is also used in Civil and Electrical Engineering, aswell as the Physics and Chemistry departments. ANSYS provides a cost-effective way to explore the performance ofproducts or processes in a virtual environment. This type of product development is termed virtual prototyping.With virtual prototyping techniques, users can iterate various scenarios to optimize the product long before themanufacturing is started. This enables a reduction in the level of risk, and in the cost of ineffective designs. The multifacetednature of ANSYS also provides a means to ensure that users are able to see the effect of a design on the whole behavior ofthe product, be it electromagnetic, thermal, mechanical etc.ANSYS is capable of both steady state and transient analysis ofany solid with thermal boundary conditions. Steady-state thermal analyses calculate the effects of steady thermal loads on asystem or component. Users often perform a steady-state analysis before doing a transient thermal analysis, to help establishinitial conditions. A steady-state analysis also can be the last step of a transient thermal analysis; performed after all transienteffects have diminished.A steady-state thermal analysis may be either linear, with constant material properties; or nonlinear, with materialproperties that depend on temperature. The thermal properties of most material vary with temperature. This temperaturedependency being appreciable, the analysis becomes nonlinear. Radiation boundary conditions also make the analysisnonlinear. Transient calculations are time dependent and ANSYS can both solve distributions as well as create video for timeincremental displays of models. The ANSYS/Multiphysics, ANSYS/Mechanical, ANSYS/FLOTRAN, and ANSYS/Thermalproducts support steady-state thermal analysis. A steady-state thermal analysis calculates the effects of steady thermal loadson a system or component. Engineer/analysts often perform a steady-state analysis before doing a transient thermal analysis,to help establish initial conditions. A steady-state analysis also can be the last step of a transient thermal analysis, performedafter all transient effects have diminished. You can use steady-state thermal analysis to determine temperatures, thermalgradients, heat flow rates, and heat fluxes in an object that are caused by thermal loads that do not vary over time. A steady-state thermal analysis may be either linear, with constant material properties; or nonlinear, with material properties thatdepend on temperature. The thermal properties of most material do vary with temperature, so the analysis usually isnonlinear. Including radiation effects also makes the analysis nonlinear.II. Literature ReviewEkrem Buyukkaya and Muhammed Cerit investigated the effects of ceramic coating over diesel engine piston using3D finite element method; they found that maximum surface temperature of the coated piston with material which has lowthermal conductivity is improved approximately 48% for the AlSi alloy and 35% for the steel.. EkremBuyukkaya,Department of Mechanical Engineering, Esentepe Campus, Turkey.. Thermal analysis of functionally graded coating AlSialloy and steel pistons... Thermal analyses were employed to deposit metallic, cermet and ceramic powders such as NiCrAl,NiCrAl+MgZrO3 and MgZrO3 on the substrate. The numerical results of AlSi and steel pistons are compared with eachother. It was shown that the maximum surface temperature of the functional graded coating AlSi alloy and steel pistons wasincreased by 28% and 17%, respectively. . Imdat Taymazinvestigated the effect of thermal barrier coatings on dieselengine performance his results indicate a reduction in fuel consumption and an improvement in the efficiency of the dieselengine.. P. M. Pierz investigated the thermal barrier coating development for diesel engine aluminum piston he found thatthe resulting predicted temperatures and stresses on the piston, together with material strength information, the primary causeof coating failure is proposed to be low cycle fatigue resulting from localized yielding when the coating is hot and incompression.. O. Altun ,Mechanical Engineering Department , Turkey., Investigated in Problems for determining thethermal conductivity of TBCs by laser-flash method., Laser-flash method is the most widely used experimental technique todetermine the thermal conductivity of APS TBCs at high temperatures. The research contributes to better understanding andrecognition the importance of sample preparation in laser-flash method.S. C. Mishra., Laser and Plasma Technology Department, Mumbai, India. Investigated in Microstructure, Adhesion,and Erosion Wear of Plasma Sprayed Alumina–Titanium Composite Coatings.. Adhesion strength value of the coating varieswith operating power. The trend of erosion of the coatings seems to follow the mechanism predicted for brittle materials.Coating deposited at 18kW power level shows a higher erosion rate than that of the sample deposited at 11kW power level. H.W. Grunling and W. Mannsmann, ABB Kraftwerrke AG, KallstadterStz 1, 6800 Mannheim 31, Germany.,investigated in Plasma sprayed thermal barrier coatings for industrial gas turbines: morphology, processing and properties.The properties of thermal barrier coating systems depend strongly on the structure and phase composition of the coatinglayers and the morphology of and the adhesion at the ceramic-metal interface. They have to be controlled by the processitself, the process parameters and the characteristics of the applied materials. . A. J. Slifka, National Institute of Standardsand Technology, Boulder. Thermal-Conductivity Apparatus for Steady-State, Comparative Measurement of CeramicCoatings, and an apparatus has been developed to measure the thermal conductivity of ceramic coatings. Since the methoduses an infrared microscope for temperature measurement, coatings as thin as 20 _m can, in principle, be measured using thistechnique. This steady-state, comparative measurement method uses the known thermal conductivity of the substratematerial as the reference material for heat-flow measurement.. Dongming Zhu Ohio Aerospace Institute, Cleveland,Ohio. Effect of Layer-Graded Bond Coats on Edge Stress Concentration and Oxidation Behavior of Thermal BarrierCoatings.. A low thermal expansion and layer-graded bond coat system, that consists of plasma-sprayed FeCoNiCrAI andFeCrA1Y coatings and a high velocity oxy fuel (HVOF) sprayed FeCrAIY coating, was developed for minimizing thethermal stresses and providing excellent oxidation resistance.. S. Alphine’, M. Derrien, Thermal Barrier Coatings: theThermal Conductivity challenge. In this paper, the importance of the challenge associated with the control of the thermal
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-1435-1441 ISSN: 2249-6645www.ijmer.com 1437 | Pageconduct why of thermal barrier coatings for turbine engines hot stages is being reviewed. It is firstly illustrated by thedescription of a practical aeronautic coated and uncoated turbine blade design exercise. The various contributions to TBCthermal conductivity are then reviewed. .III. Thermal Barrier CoatingThermal barrier coatings are highly advanced material systems applied to metallic surfaces, such as gas turbineaero-engine and diesel engine parts, operating at elevated temperatures. These coatings serve to insulate metallic componentsfrom large and prolonged heat loads by utilizing thermally insulating materials which can sustain an appreciable temperaturedifference between the load bearing alloys and the coating surface. In doing so, these coatings can allow for higher operatingtemperatures while limiting the thermal exposure of structural components, extending part life by reducing oxidation andthermal fatigue. In fact, in conjunction with active film cooling, Thermal barrier coatings permit flame temperatures higherthan the melting point of the metal airfoil in some turbine applications.Modern Thermal barrier coatings are required to notonly limit heat transfer through the coating but to also protect engine components from oxidation and hot corrosion. Nosingle coating composition appears able to satisfy these multifunctional requirements. As a result, a “coating system” hasevolved. Research in the last 20 years has led to a preferred coating system consisting of three separate layers such as metalsubstrate, bond coat and ceramic coating to achieve long term effectiveness in the high temperature, oxidative and corrosiveuse environment for which they are intended to function.The application of Thermal barrier coatings on the diesel engine piston head reduces the heat loss to the enginecooling-jacket through the surfaces exposed to the heat transfer such as cylinder head, liner, piston crown and piston rings. Itis important to calculate the piston temperature distribution in order to control the thermal stresses and deformations withinacceptable levels. The temperature distribution enables the designer to optimize the thermal aspects of the piston design atlower cost, before the first prototype is constructed. As much as 60% of the total engine mechanical power lost is generatedby piston ring assembly. Most of the internal combustion (IC) engine pistons are made of aluminum alloy which has athermal expansion coefficient 80% higher than the cylinder bore material made of cast iron. This leads to some differencesbetween running and the design clearances. Therefore, analysis of the piston thermal behavior is extremely crucial indesigning more efficient engines. The thermal analysis of piston is important from different point of views. First, the highesttemperature of any point on piston should not exceed 66% of the melting point temperature of the alloy. This limitingtemperature for the current engine piston alloy is about 370°C. This temperature level can be increased in ceramic coatingdiesel engines.Thermal barrier coatings consist of three layers. They are the metal substrate, metallic bond coat and ceramictopcoat. The metal substrate and metallic bond coat are metal layers and the topcoat is the ceramic layer. The metal substrateis typically a high temperature aluminium alloy that is either in single crystal or polycrystalline form. The metallic bond coatis an alloy typically with the composition of Nickel, Cobalt, Chromium, Aluminium. The bond coat creates a bond betweenthe ceramic coat and substrate. The third coat is the ceramic topcoat, Zirconia (ZrO3), Mullite(3Al2O3-2SiO2), Alumina(Al2O3) which is desirable for having very low conductivity while remaining stable at nominal operating temperaturestypically seen in applications. This layer creates the largest thermal gradient of the thermal barrier coating. In industry,thermal barrier coatings are produced in a number of ways. Electron Beam Physical Vapor Deposition (EBPVD) Air Plasma Spray (APS) Electrostatic Spray Assisted Vapour Deposition (ESAVD) Direct Vapor DepositionDiesel engine piston made of Aluminium Alloy is taken for this study and ceramic material having low thermalconductivity is preferred as the coating material on the piston head or crown.Fig.1. Materials for thermal barrier coating
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-1435-1441 ISSN: 2249-6645www.ijmer.com 1438 | PageThe ceramic material choosen for this study should have low thermal conductivity and thermal expansion as shownin the above graph. The selected materials are as follows, Zirconia (ZrO2) Mullite (3Al2O3-2SiO2) Alumina (Al2O3)IV. Electron Beam Physical Vapor DepositionEB-PVD is an evaporation process for applying ceramic thermal barrier coatings to gas turbine engine parts .It hasbeen the favored deposition process technique for TBCs because of the increased durability of coating that is produced whencompared to other deposition processes. EB-PVD TB exhibits a columnar microstructure that provides outstanding resistanceagainst thermal shocks and mechanical strains. Figure presents a diagram of the coating chamber where the EB-PVD processtakes place.The EB-PVD process takes place in a vacuum chamber consisting of a vacuum-pumping system, horizontalmanipulator, a water-cooled crucible containing a ceramic ingot to be evaporated, an electron-beam gun, and the work piecebeing coated. The electron beam gun produces electrons, which directly impinge on the top surface on the ceramic coating,located in the crucible, and bring the surface to a temperature high enough that vapor steam is produced. The vapor steamproduces a vapor cloud, which condenses on the substrate and thus forms a coating. The substrate is held in the middle ofvapor cloud by a horizontal manipulator that allows for height variation in the chamber. During the coating process, oxygenor other gases may be bled into the vapor cloud in order to promote a stoichiometric reaction of ceramic material. An .oversource.heater or an electron beam gun may be used for substrate heating, which keeps the substrate at a desired temperature.Figure 2. EB-PVD Coating ChamberIn our six stroke engine we are placing thermal barrier component in between the cylinder block and cylinder liner.The heat is transferred from the combustion chamber to the cylinder block through the cylinder liner and thermal barrier. Theheat flow rate through the thermal barrier is low. Materials of thermal barrier are discussed in the forthcoming chapters.V. SimulationIn this project work, ANSYS workbench 10 software has been used to investigate the temperature distribution in theceramic coated Aluminium alloy piston and to compare the maximum surface temperature of the uncoated Aluminium alloypiston with ceramic coated Aluminium alloy piston, ceramic materials such as Zirconia stabilized with magnesium oxide,Mullite and Alumina were used for this studyIn the numerical simulation performed, a diesel engine piston, made of Al alloy is analyzed. 3-D finite elementthermal analyses are carried out on both uncoated and ceramic coated pistons. In the model, surface-to-surface contactelements are defined between piston ring and ring grove. Piston thermal boundary conditions consist of the ring land andskirt thermal boundary condition, underside thermal boundary condition, combustion side thermal boundary condition.Convective heat transfer coefficients and ambience temperatures were specified as the thermal boundary conditions.Fig 3. Thermal circuit of heat transfer resistances in the region of the rings.
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-1435-1441 ISSN: 2249-6645www.ijmer.com 1439 | PageR1: Conductive resistance of the ring,R2: Conductive resistance of the oil film is negligible,R3: Conductive resistance of the liner,R4: Convective resistance between the liner and the cooling water.Thermal circuit of heat transfer resistances in the ring land is to be set with the following assumptions.1) The effect of piston motion on the heat transfer is neglected.2) The rings and skirt are fully engulfed in oil and there are no cavitations.3) The rings do not twist.4) The heat transfer mode in the oil film is neglected.Table .1.Thermal properties of partsMaterial Thermal conductivityW/m0CPiston (Al-Si) 155Oil Ring 33Compression Ring 52Liner 55The resistances are:Conductive resistance of the ring, R1=(ln(r1/r2)/2пL1Kring) = 0.085048 m2k/kwConductive resistance of the film, R2=(ln(r3/r2)/2пL2Koil) = 8x10-5m2k/kwConductive resistance of the liner, R3=(ln(r4/r3)/2пL3Kblock) = 0.06417 m2k/kwConductive resistance between the liner and cooling water, R4 = 1/ (hwaterAs) =0.171 m2k/kwTotal resistance Rtot=0.32 m2k/kwThe effective heat transfer is obtained from, heff=1/RtotxAeff = 617.68 w/m2kThe value of convective heat transfer coefficient of crown underside is, hun1=900(N/4600)0.35=672.415 w/m2kThe value of convective heat transfer coefficient of piston skirt underside, hun2=240(N/4600)0.35=179.31 w/m2kThe Crevice heat transfer coefficient, h=k/S =230 w/m2kTable 2.Coating MaterialsPropertiesAluminium-Silicon AlloyZirconia stabilized withMagnesium oxide (ZrMgO3)Mullite(3Al2O3•2SiO2)Alumina(Al2O3)Density kg/m³ 2.68 x10³ 5.6 x10³ 2.8 x10³ 3.69 x10³Thermal expansion (20 ºC) ºCˉ¹ 19.4x10-610x10-65.4x10-67.3x10-6Specific heat capacity J/(kg*K) 850 400 950 880Thermal conductivity W/(m*K) 154 2.5 6 18Initial ConditionsPiston top surface temperature : 4000CPiston skirt temperature : 1100CBoundary ConditionsThe Crevice convective heat transfer coefficient, h = 230 w/m2kThe piston crown or head underside convective heat transfer coefficient,hun1 = 672.415 w/m2kThe piston skirt underside convective heat transfer coefficient, hun2 = 179.31 w/m2kFig .4 Uncoated Aluminium alloy piston Fig 5.Ceramic material Zirconia coated piston
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-1435-1441 ISSN: 2249-6645www.ijmer.com 1440 | PageFig .6 Ceramic materialMullite coated piston Fig 7. Ceramic material Alumina coated pistonVI. Results and DiscussionFinite element analysis were performed to evaluate temperature gradients of the uncoated Aluminium alloy pistonand ceramic materials such as partially stabilised zirconia with magnesium oxide (ZrMgO3), Mullite and Alumina (Al2O3)coated Aluminium alloy piston. The temperature distributions of an uncoated aluminium alloy piston are shown in the figure4. The maximum surface temperature on the piston crown of the Aluminium alloy piston is determined as 295.860C.Thetemperature distributions of the ceramic materials such as partially stabilised zirconia with magnesium oxide (ZrMgO3),Mullite and Alumina (Al2O3) coated Aluminium alloy piston is shown in the figure 5, figure 6, figure7, respectively.Themaximum surface temperature on the piston crown for Ziconia coated Aluminium alloy piston is determined as 377.070C,For Mullite Coating it is 360.60C and for Alumina coating it is 357.450C.Fig.8 represents the temperature distribution comparison curve of uncoated Aluminium alloy piston with zirconia,Mullite and Alumina coated piston. It is clear that the maximum surface temperature of Zirconia coated piston (377.070C) ismore than the conventional Aluminium alloy piston (295.860C).and the maximum surface temperature of Mullite coatedpiston (360.60C) is more than the conventional Aluminium alloy piston (295.860C) and the maximum surface temperature ofAlumina coated piston (377.070C) is more than the conventional Aluminium alloy piston (295.860C).From the graphicalrepresentation the ceramic material partially stabilized Zirconia gives more performance to the diesel engine taken for thisstudy.Fig. 8.Comparisons of coated Aluminium alloy piston with uncoated Aluminium alloy pistonVII. ConclusionA comparative evaluation was made between the temperature distributions of the uncoated aluminium alloy pistonand the ceramic coated piston. The maximum surface temperature of the ceramic coated piston is improved approximately28% for Zirconia stabilised with magnesium oxide (ZrMgO3) coating, 22% for Mullite coating (3Al2O3-2SiO2) and 21% forAlumina (Al2O3) than the uncoated piston by means of ceramic coating. According to the software simulations conducted inthis project, it has been concluded that the using of ceramic coating for Aluminium alloy piston increases the temperature ofthe combustion chamber of the engine and the thermal strength of the base metal.Finally the combustion chambertemperature increases the thermal efficiency of the engine also increases.
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-1435-1441 ISSN: 2249-6645www.ijmer.com 1441 | PageReferences. EkremBuyukkaya, (2008) Thermal analysis of functionally graded coating AlSi alloy and steel pistons.. EkremBuyukkaya, MuhammetCerit, (2008) Thermal analysis of a ceramic coating diesel engine piston using 3-D finite elementmethod.. Imdat Taymaz, (2006) the effect of thermal barrier coatings on diesel engine performance.. P.M. Pierz, (1993) Thermal barrier coating development for diesel engine aluminium pistons.. O. ALTUN, Investicated in Problems for determining the thermal conductivity of TBCs by laser-flash method. S. C. MISHRA., investigated in Microstructure, Adhesion, and Erosion Wear of Plasma Sprayed Alumina–Titanium CompositeCoatings. H.W. GRUNLING and W. MANNSMANN, ABB Kraftwerrke AG, KallstadterStz 1, 6800 Mannheim 31, Germany., Investigated inPlasma sprayed thermal barrier coatings for industrial gas turbines: morphology, processing and properties. A. J. SLIFKA, National Institute of Standards and Technology, Boulder. Thermal-Conductivity Apparatus for Steady-State,Comparative Measurement of Ceramic Coatings. DONGMING ZHU Ohio Aerospace Institute, Cleveland, Ohio. Effect of Layer-Graded Bond Coats on Edge Stress Concentrationand Oxidation Behavior of Thermal Barrier Coatings.. S. Alphine’, M. Derrien*, A review of Thermal Barrier Coatings for turbine.Authors Bibliography:K. Sridhar-received his B.E., Degree in Mechanical Engineering from Anna University, Chennai. He receivedM.E. Degree from ANNA University, Coimbatore. Currently working as a teaching faculty in the School ofMechanical and Industrial Engineering, Institute of Technology, Bahir Dar, University, Bahir Dar, Ethiopia.R.Rejikumar received his B.E., Degree in Mechanical Engineering from Anna University, Chennai. He receivedM.E. Degree from ANNA University, Thiruchirapalli. Currently working as a teaching faculty in the School ofMechanical and Industrial Engineering, Institute of Technology, Bahir Dar, University, Bahir Dar, EthiopiaMr. M. Narasimha received his B.Tech. Degree in Mechanical Engineering from JNTU, Hyderabad, India. Hereceived M.E. Degree from VMU, TAMILNADU; currently working as a teaching Faculty in the School ofMechanical and Industrial Engineering, Institute of Technology, Bahir Dar University, Bahir Dar, Ethiopia.